Wear Inducing Phase Transformation of Plasma Transfer Arc ... Wear Inducing Phase Transformation of
Embed Size (px)
Transcript of Wear Inducing Phase Transformation of Plasma Transfer Arc ... Wear Inducing Phase Transformation of
Research Article Wear Inducing Phase Transformation of Plasma Transfer Arc Coated Tools during Friction Stir Welding with Al Alloy
Kuan-Jen Chen ,1 Fei-Yi Hung ,2 Truan-Sheng Lui,2 and Yong-Ren Shih2
1The Instrument Center, National Cheng Kung University, Tainan 701, Taiwan 2Department of Materials Science and Engineering, National Cheng Kung University, Tainan 701, Taiwan
Correspondence should be addressed to Fei-Yi Hung; firstname.lastname@example.org
Received 9 August 2018; Accepted 26 November 2018; Published 1 January 2019
Guest Editor: Long Wan
Copyright © 2019 Kuan-Jen Chen et al.This is an open access article distributed under the Creative Commons Attribution License, which permits unrestricted use, distribution, and reproduction in any medium, provided the original work is properly cited.
The friction stir welding process (friction stir welding/processing, FSW/FSP) has wear problems related to stirring tools. In this study, the plasma transfer arc (PTA) method was used with stellite 1 powders (Co-based) to coat on the head of a SKD61 stirring tool (SKD61-ST1) in order to investigate the wear performance and phase transformation of SKD61-ST1 after FSW. Under the same experimental parameters, thewear datawere comparedwith the high-speed steel SKH51 (temperingmaterial SKH51-T andannealed material SKH51-A) and tungsten-carbide cobalt (TCC). Results showed the PTA coating was a 𝛾-Co solidificationmatrixwithM
7 C 3
and M 23 C 6 carbides. After FSW, the wear resistance of SKD61-ST1 was better than that of SKH51-A and SKH51-T and lower than
that of TCC. The SKD61-ST1, SKH51-A, and SKH51-T stirring tools exhibited sliding wear after FSP, where the pin and shoulder of the stirring tool formed a phase transfer layer on the surface, and the peeling of the phase transfer layer caused wear weight loss. The main phase of the phase transfer layer of the SKD61-ST1 tool was Al
9 Co 2 . The affinity and adhesion energy of the Co-Al phase
was lower than that of Fe-Al phase, and the phase transfer layer of the SKD61-ST1 tool was thinner and had lower coverage, thereby increasing the wear resistance of the SKD61-ST1 stirring tools during FSW.
Temperature of friction stir welding (FSW) occurs under the melting point of metal and thus can prevent typical solidification defects of traditional joining methods . FSW can induce frictional heat and plastic metal flow, generat- ing dynamic recrystallization, grain refinement, and second phase refinement that enhances the mechanical properties of materials [2, 3].
In recent years, FSW has been widely used in Al alloys, but the stirring rods have wear problems and reduce the life of the stirring rods [4–6]. Tungsten carbide (WC) is extremely hard; therefore tools are often made with WC and cobalt alloy powders to form high wear-resistance tungsten-carbide cobalt (TCC) materials using a sintering process. The use of a TCC stirring rod can increase wear performance and life, but it is expensive. Therefore, developing a new stirring tool that meets the need for appropriate wear conditions and affordability is necessary. SKH51 is one of themost commonly
used high-speed tool steels. Under high-speed conditions, it can still maintain goodmechanical properties, and its price is lower than that of TCC, so it is often used as a stirring tool in FSW .
The SKD61 is a tool steel with good thermal-crack resistance, and it is cheaper than SKH51 . Coating on the pin of an SKD61 stirring rod for FSW causes a better wear resistance. The plasma transferred arc (PTA) process is a surface coating treatment [9, 10]. The plasma arc between the electrode and the substrate is used to coat the alloy powders on the substrate to form a highly wear resistant coating layer. PTA has many characteristics: (1) The PTA- overlay is thicker than a laser induced overlay. Because the PTA-overlay is metallurgical bond, its impact-resistance is higher. (2) The powder can be selected at random, and the composition of the overlayer can be established easily. (3)The working distance between the electrode and work-surface is more flexible. The PTA process has higher work efficiency and is commonly used in surface-overlaid manufacturing.
Hindawi Journal of Engineering Volume 2019, Article ID 6413608, 10 pages https://doi.org/10.1155/2019/6413608
http://orcid.org/0000-0002-9624-221X http://orcid.org/0000-0001-5432-0980 https://creativecommons.org/licenses/by/4.0/ https://doi.org/10.1155/2019/6413608
2 Journal of Engineering
19.3 mm SKD
Stellite 1 (overlayer)
3~4 mm 1 mm
Figure 1: Stellite overlayer processing to the pin and shoulder.
In addition, stellite 1 powders had good wear resistance and thermal shock properties and therefore are often used as a coating material .
For above reasons, this study used PTA process to coat stellite 1 powders on SKD61 alloy steel to form the stirring tool (SKD61-ST1). The coating structure of the SKD61-ST1 tool was investigated and also used in FSW for a 5083 aluminum alloy substrate to discuss the wear characteristics. Notably, the stirring wear rates of SKH51 high-speed steels (annealed SKH51-A and tempering SKH51-T) and TCC were compared with SKD61-ST1 under the same experimental parameters. In addition, the wear mechanism (wear induced phase transformation) of SKD61-ST1 was investigated. The phase transformation of the stirring tool can confirm thewear fracture characteristics, and the correlation data may serve as a reference for the application of a FSW system.
2. Experimental Procedure
2.1. Stirring Tool Preparation. PTA coated stellite 1 powders were used on the surface of SKD61 mold steel to form an SKD61-ST1 stirring rod. SKH51 high-speed steel (SKH51- A) was annealed, underwent oil quenching, and was then tempered to form an SKH51 high-speed steel tempering material (SKH51-T: oil quenching at 1230∘C for 4 minutes; tempering at 560∘C for 2 hours). This experiment involved the use of four stirring rods: (1) SKD61-ST1, (2) SKH51-A, (3) SKH51-T, and (4) TCC. FSW performed four rods in a 5083 aluminum alloy substrate in order to acquire the wear data for the stirring rods under the same experimental parameters. After the FSW, the pin edge of the stirring rod was observed, and the hardness of the head of the stirring rod was measured. Scanning electron microscopy (SEM), energy dispersive spectroscopy (EDS), electron probe X- ray microanalyzer (EPMA), and X-ray diffraction (thin film XRD) were used to investigate the wear characteristics and wear induced phase transformation.
Figure 2: OMmetallurgical phase of the SKD61 annealing material.
2.2. Coating of the SKD61 Tool Using the PTA Process. Stellite 1 powders were coated on the head of the SKD61 stirring rod, the thickness of the stellite 1 overlayer was 3∼4 mm. To polish the stellite 1 overlayer, a pin with a height of 1 mm and a diameter of 5 mm was formed on the surface of the shoulder with a diameter of 19.3 mm. A schematic diagram of the SKD61-ST1 stirring rod is shown in Figure 1. Notably, the pin, shoulder, and friction stir zone were SKD61-ST1 (stellite 1 overlayer structure). In addition, SKD61 matrix was an annealed structure and the hardness was about 24 HRC. The microstructure and chemical composition are shown in Figure 2 and Table 1. The chemical composition of stellite 1 powders is provided in Table 2, and the PTA experimental parameters are shown in Table 3.
2.3. Wear Measurement and Subsurface Observation of the Stirring Rod. The SKD61-ST1, SKH51-A, SKH51-T, and TCC stirring rods were the same size (Figure 1) and underwent the friction stir test under the same experimental parameters.The stirred substrate was the annealed 5083 aluminum alloy, and the walking distance for every stirring rod was five meters (each walk was 0.5m, which was then stopped and cooled for
Journal of Engineering 3
Table 1: Chemical composition of the SKD61 mold steel (PTA coated substrate) (wt.%).
C Si Mn P S Cr Mo V Fe 0.35 0.80 0.40 0.02 0.02 4.50 1.20 1.00 Bal.
Pin 5083 alloy
Figure 3: Schematic diagram of the friction stir process.
Table 2: Chemical composition of the stellite 1 cobalt-based alloy (PTA coating powder) (wt%).
Cr C W Si Co 32.00 2.50 11.50 2.00 Bal.
Table 3: PTA process parameters.
Powder flux 1200 g/hr Plasma gas (Ar) 4 l/min Powder delivery gas (Ar) 3 l/min Shielding gas (Ar) 24 l/min Overlay current 90A Overlay voltage 36V
Table 4: The friction stir process (FSP) parameters.
Stirring rod speed 1256 RPM Specimen feed rate 4 mm/s Stirring rod tilt angle 1.5∘
Under pressure 43.4 MPa Stirred material Annealed 5083 Al alloy Stirred substrate size 150 × 46 × 13 mm3
Walking distance 5 m
five minutes, and repeated 10 times). The speed and feed rate of the stirring rod were 1256 rpm and 4 mm/s, respectively. Theparameters for the FSW test are shown inTable 4. Figure 3 is a schematic diagram of the FSW. The microstructure and chemical composition of the 5083 aluminum alloy are shown in Figure 4 and Table 5.
Before and after the FSW, the weight of stirring rod was measured to obtain the wear rate. After the FSW, the head of the stirring was adhered to the 5083 aluminum alloy, so the stirring head was put into an aqueous solution of 50
wt.%NaOH to remove the 5083 aluminum alloy and then the weight loss was measured.
2.4. Observation of Wear Subsurface. After the FSW, the pin and shoulder of the SKH51-A, SK